## mixed-mode parameters

Matthew Robert Molteno*Dissertation presented for the degree of Doctor of Philosophy *
*in the Faculty of Engineering at Stellenbosch University *

Supervisor: Thorsten Hermann Becker

i

Declaration

By submitting this dissertation electronically, I declare that the entirety of the work contained therein is my own, original work, that I am the sole author thereof (save to the extent explicitly otherwise stated), that reproduction and publication thereof by Stellenbosch University will not infringe any third-party rights and that I have not previously in its entirety or in part submitted it for obtaining any qualification.

Date: December 2017

M.R. Molteno

Copyright © 2017 Stellenbosch University All rights reserved

ii

## Abstract

The degradation of material properties over time is one of the core constituents of structural
integrity monitoring. For this purpose, the materials’ resistance to brittle fracture is the most widely
used property in the determination of safe operation and predicting component life. Measuring
such properties by conventional methods presents challenges: large numbers of samples are
needed, accounting for mixed-mode loading. Non-contact measurements by digital image
correlation shows promise in extracting such parameters from *in situ* loaded structures, accounting
for their complex geometry and loading.

This thesis aims to develop a framework that allows for the extraction of mixed-mode brittle
fracture properties, using three-dimensional (3D) image correlation techniques: multi-camera
Digital Image Correlation (stereo-DIC), and Digital Volume Correlation (DVC). The 𝐽-integral
method was chosen for obtaining the fracture resistance, with the decomposition method used for
determining separate 𝐽_{𝐼−𝐼𝐼𝐼} components (opening, sliding and shearing: modes I, II and III), and
stress intensity factors (𝐾𝐼−𝐼𝐼𝐼), as both methods are resilient to crack tip and displacement errors.

The first stage of development is a finite element based method for the removal of experimental displacement artifacts from DIC or DVC results, intended as a pre-processor for the 𝐽-integral. Subsequently, a theoretical derivation is provided to link the two volumetric forms: the volume and the path-area integrals. This results in a proposed ‘hybrid’ integral, which benefits from the resilience to crack-front positional errors of the path-area approach, and resilience to random displacement noise of the volume integral.

Initial testing of the 𝐽-integral based decomposition method was on the surface using stereo-DIC and the Arcan fixture to induce mixed-mode loading. The results are verified with mixed-mode fracture toughness values measured from PMMA and compared to literature and ASTM 1820 tests. The typical image correlation errors close to fracture are quantified by a methodology of applying the 𝐽-integral to analytical crack tip fields to which displacement errors are added artificially. It was found that the 𝐽-integral is most prone to DIC errors under anti-symmetric (mode II/III) loading.

Testing in the volume used X-ray computed tomography to acquire images and DVC for displacement maps. The measurements were verified on two configurations: a SENT polyurethane composite specimen (mode I), and a shear loaded inclined notch in Magnesium alloy-WE43 (mixed-mode). The 𝐽-integral was verified against values from finite element fields resulting again in larger errors in mixed-loading. Decomposition of the volume integral requires an approach to separate the anti-symmetric 𝐽-integral. Two extensions are proposed: the first using a ratio derived from mode II/III Williams series formulas, and the second using the interaction integral. Both approaches are verified on DVC displacements.

This thesis finds that 𝐽 based decomposition offers a versatile method to extract 𝐾_{𝐼−𝐼𝐼𝐼} values from
non-standard 3D geometries and loadings. However, the pre-processing of fields to minimise
errors is essential when mode II-III displacement fields are prominent.

Although it is beyond the scope of this thesis, the hope is that this work will assist in the adoption of full-field measurement techniques as a standard testing practice in structural integrity assessments, and lead to better informed maintenance and inspection schedules.

iii

## Opsomming

Die agteruitgaan van material-eienskappe met tyd is een van die kernkomponente van strukturele
integriteit monitering. Vir hierdie doel is die materiaal se weerstand teen brosfraktuur die mees
algemene gebruikte eienskap vir die bepaling van veilige werking en die voorspel van die
komponent se leeftyd. Die meet van sulke eienskappe volgens konvensionele metodes bied
uitdagings, bv. groot getalle monsters word benodig en komplekse kragte moet in ag geneem word.
Nie-kontakmetings deur digitale-beeldkorrelasie toon belofte om sulke parameters uit *in situ*

gelaaide strukture te onttrek, terwyl komplekse kragte en material vorme in ag geneem word.
Hierdie proefskrif beoog om 'n raamwerk te ontwikkel wat die ontginning van gemengde-modus
brosfraktuur-eienskappe moontlik maak deur gebruik te maak van driedimensionele (3D)
beeldkorrelasietegnieke: Digitale Kamera-Korrelasie (stereo-DKK) en Digitale Volume
Korrelasie (DVK). Die 𝐽-integrale metode is gekies vir die verkryging van die breukweerstand,
met behulp van die ontbindingsmetode vir die bepaling van afsonderlike 𝐽_{𝐼−𝐼𝐼𝐼} komponente
(opening, gly en skeer: mode I, II en III) en stresintensiteitsfaktore (𝐾𝐼−𝐼𝐼𝐼), aangesien beide

metodes skerm teen kraakpunt en verplasings foute.

Die eerste fase van ontwikkeling is 'n eindige element gebaseerde metode vir die verwydering van eksperimentele verplasing artefakte van DKK of DVK resultate, wat bedoel is as 'n voorverwerker vir die 𝐽-integraal. Vervolgens word 'n teoretiese afleiding verskaf om die twee volumetriese vorms te verbind, naamlik die volume en pad-area integrale. Dit lei tot 'n voorgestelde 'hibriede'-integraal. Hierdie ‘hibriede’-integraal vereis ‘n kompromie tussen die robuustheid van die pad -area-benaderingsfout van die pad-area-benadering en robuustheid van lukrake verplasings geraas van die volume-integraal.

Aanvanklike toetsing van die 𝐽-integraal gebaseerde ontbindings metode is op die oppervlak met behulp van stereo-DKK, en die Arcan greep om gemengde-mode laai te veroorsaak. Die resultate word geverifieer met gemengde-mode-fraktuur taaiheid waardes, gemeet vanaf PMMA en baseer op literatuur sowel as die ASTM 1820 toetse. Die tipiese beeldkorrelasie foute naby aan fraktuur word gekwantifiseer deur die toepassing van die 𝐽-integraal op analitiese kraakpuntvelde waarby verplasingsfoute kunsmatig bygevoeg word. Daar is bevind dat die 𝐽-integraal die meeste geneig is tot DKK foute onder asimmetriese (mode II/III) laai.

Toets in die volume gebruik X-straal-rekenaartomografie om beelde en DVK vir verplasings
kartering te bekom. Die metings is geverifieer op twee konfigurasies: 'n SENT
saamgestelde-polyuretaan monster (mode I) en 'n skuinsbelaaide spleet in magnesium-allooi, WE43 (gemengde
mode). Die 𝐽-integraal is geverifieer teen waardes van eindige elementvelde wat weer groter foute
in gemengde laai veroorsaak. Ontleding van die volume-integraal vereis 'n benadering om die
anti-simmetriese 𝐽-integraal te skei. Twee uitbreidings word voorgestel: die eerste met behulp van 'n
verhouding wat afgelei word vanaf mode II / III Williams reeks formules, en die tweede maak
gebruik van die interaksie integraal. Albei benaderings word geverifieer op DVK-verplasings.
Hierdie proefskrif bevind dat 𝐽 gebaseerde ontbinding 'n veelsydige metode bied om 𝐾_{𝐼−𝐼𝐼𝐼}

waardes uit nie-standaard 3D-geometrieë en ladings te onttrek. Die voorbereiding van velde om foute te beperk, is egter noodsaaklik wanneer die mode II-III verplasingsvelde prominent is. Alhoewel dit buite die omvang van hierdie proefskrif is, is die hoop dat hierdie werk sal help met die aanvaarding van volwaardige metingstegnieke as 'n standaard toetspraktyk in strukturele integriteit assesserings, en lei tot beter ingeligte onderhouds en inspeksieskedules.

## Acknowledgements

My heartfelt acknowledgement goes to Dr Thorsten Becker whose expertise, vision, and leadership were a constant inspiration; and whose kindness and foresight guided this work through diverse terrains. Secondly, I sincerely thank Prof. James Marrow, whose insights, supervision and support significantly contributed to the development of this thesis, and who made me feel very welcome in Oxford.

I would also like to thank my defense committee: Prof. Fabrice Pierron, Prof. Satoru Yoneyama and Prof. Gerhard Venter, for their insightful comments, encouragement, and probing questions.

My deepest gratitude goes to my parents, Martin and Jane for their understanding and support through each of my post-graduate endeavors. Thanks also goes to my brothers: Steve, Robin, and Chris, for keeping me motivated.

Thank you to Marisa Storm for her unwaivering love and support during the doctoral journey. To Dr Robert Pott, thank you for leaving food out for the nocturnal creature that took up residence in your house during the final stages of write-up. To Uri Bram, Mieke du Plessis, Joelle Grogan, Anna Frangou, Teddy Rose (TR) Stegmann, Daan Henselmans, and Lily Prollius; thank you for whisking me away from my thesis when it was most needed. Thanks are also extended to the research groups I have attended who provided encouragement, and many laughs. In the Stellenbosch group: Richard Huchzermeyer, Nur Dhansay, Sergey Petrov, Lucas Anderson, Devan Atkinson, Melody van Rooyen, Arno Scholtz and Gerrit ter Haar; in the Oxford group: Matthew Jordan, Selim Barhli, Ahmet Cinar, Yelena Vertyagina and Luis Saucedo Mora.

It is also essential to mention the staff who greatly enlivened my time at Stellenbosch University with their dedication and general positivity. In particular, I would like to thank Ms Welma Liebenberg, Prof. Gerhard Venter, Dr Martin Venter and Prof. Thomas Harms. Importantly, I would like to acknowledge the NRF-Thrip fund for the financial support, as well as the ESKOM EPPEI programme for the bi-yearly meetings, and valuable input from industry.

## Table of contents

**Page**

**Declaration ... i**

**Abstract ... ii**

**Opsomming ... iii**

**Acknowledgements ... 5**

**Table of contents ... 6**

**List of figures ... 9**

**List of tables ... 13**

**List of abbreviations ... 14**

**Nomenclature ... 15**

**1**

**Background reading ... 20**1.1 Project background ... 21

1.2 Full-field measurements with image correlation ... 22

1.3 The role of fracture mechanics in damage evaluations ... 23

1.4 Summary of aims ... 24

1.5 Details of thesis layout ... 25

### 2 Background reading ... 26

2.1 Image correlation ... 26

2.1.1 Overview of principles ... 26

2.1.2 Displacement accuracy and spatial resolution ... 31

2.1.3 Global vs. local approaches to image correlation ... 31

2.1.4 Digital volume correlation ... 32

2.2 Damage and fracture mechanics ... 34

2.2.1 Overview of principles ... 34

2.2.2 Full-field fracture mechanics ... 36

2.2.3 Computation of energy release rates ... 37

2.2.4 The field fitting approach ... 38

2.2.5 The 𝐽-integral ... 42

2.2.6 The decomposition method ... 48

2.3 Extracting material properties from displacements ... 49

2.3.1 Optimisation based approaches ... 50

2.3.2 The virtual field method ... 51

2.4 Summary ... 53

### 3 Hypothesis development ... 54

3.1 Justification for choice of techniques ... 54

3.2 Aims and objectives ... 55

3.3 Central hypothesis ... 56

3.4.1 Non-destructive testing and evaluation ... 57

3.4.2 Experimental errors from image correlation ... 57

3.4.3 Linear-elastic deformations ... 57

3.4.4 Nominal loading ... 58

3.4.5 Spatial resolution ... 58

**4** **Robust removal of displacement artifacts from digital image and volume **
**correlation results ... 59**

4.1 Introduction ... 61

4.2 Identification of unreliable data ... 62

4.2.1 Finite element framework ... 63

4.2.2 Iterative procedure for artifact removal ... 65

4.3 Example: cantilever beam ... 68

4.4 Applications to experimental results ... 71

4.4.1 Application to DIC data ... 71

4.4.2 Application to DVC data ... 73

4.5 Discussion ... 75

4.6 Summary ... 75

### 5 Linking the path-area and volume integral approaches: a hybrid 𝑱-integral formulation ... 76

5.1 Introduction ... 77

5.2 Derivation of a volumetric form of the path-area integral ... 78

5.3 A hybrid path-area - volume integral ... 81

5.4 Review of developments ... 82

5.5 Example on numerical fields ... 83

5.6 Discussion ... 87

5.7 Summary ... 87

**6** **Mode I-III decomposition of the 𝑱-integral from DIC displacement data ... 89**

6.1 Introduction ... 90

6.2 Theoretical framework ... 92

6.2.1 The classical 𝐽-integral ... 92

6.2.2 Mode decomposition of J ... 92

6.2.3 The area integral ... 94

6.3 Validation using analytical fields ... 95

6.3.1 Implementation on analytical fields ... 95

6.3.2 𝐽-integral implementation ... 96

6.3.3 Error analysis procedure ... 97

6.3.4 Study of synthetic DIC measurement errors ... 98

6.4 Experimental implementation ... 101

6.4.1 Material and specimens ... 102

6.4.2 Fixture ... 102

6.4.4 Mixed loading results ... 105

6.5 Conclusions ... 105

6.6 Summary ... 106

### 7 Evaluation of the hybrid volume 𝑱-integral on DVC displacement data ... 107

7.1 Introduction ... 109

7.2 Three-dimensional framework ... 111

7.3 Verification on analytical fields ... 112

7.3.1 Implementation on analytical fields ... 112

7.3.2 Study of synthetic errors in three-dimensional data ... 113

7.4 Verification on DVC obtained displacement fields ... 118

7.4.1 Mode I loading: SENT specimen ... 121

7.4.2 Mixed mode experiment: inclined crack under shear loading ... 124

7.5 Conclusions ... 128

7.6 Summary ... 129

### 8 Application of the decomposition method to the volume integral and DVC data ... 130

8.1 Introduction ... 131

8.2 Decomposition in the volume: historical perspectives ... 131

8.3 The decomposition of DVC displacements ... 133

8.4 Application to finite element data ... 134

8.4.1 Discussion ... 136

8.4.2 Proposed extensions ... 138

8.5 Application to experimental data ... 142

8.6 Conclusions ... 143

8.7 Summary ... 144

**9** **Discussion ... 145**

9.1 Introduction ... 145

9.2 Minimisation of displacement errors ... 145

9.3 Evaluation of the 𝐽-integral ... 148

9.4 Decomposition from displacement fields ... 149

9.5 Future work ... 151

9.6 Recommendations for Eskom ... 151

### 10 Conclusions ... 153

**References ... 154**

**Appendix: Formulation of the surface-volume integral (𝐽s-vol) from the volume **
**integral ... 167**

## List of figures

**Page **

Figure 1.1: Life expenditures of the current coal-fired Eskom power plants (Molokwane, 2014) ... 22 Figure 1.1: (a) Crack sample (CT specimen) loaded in tension, (b) images from before

(top) and after (bottom) loading in the crack tip co-ordinate system, used as the reference and deformed configurations respectively on the surface (c) –

schematic (d) shows typical subset parameters relative to fracture ... 28 Figure 1.2: Examples of fundamental problems in image matching: (a) loss of pattern

fidelity and (b, c) the correspondence problem. (a) shows an example of stress corrosion cracking in a laser etched sample from (Becker et al., 2016), (b) is a repeating structure and (c) is a textureless deforming structure. ... 30 Figure 1.3: Typical laboratory X-CT setup of the source, rotating and translating sample,

and detector ... 33 Figure 1.4: The various defect sizes involved in fatigue and the two definitions, from Ref.

(Chaboche, 2006) ... 34 Figure 1.5: Representation of the three fracture modes: opening (mode I), shearing (mode

II), and tearing (mode III). Image from (Kuna, 2013a) ... 36 Figure 1.6: Planar crack tip co-ordinate system of point Р, and reflected point Р’ ... 40 Figure 1.7: 𝐽 path integral with contour (𝛤) looping the crack front, and local co-ordinate

system (𝑥𝑖) at crack front position s ... 43

Figure 1.8: 𝐽-integral contour Γ, and local crack co-ordinate system 𝑥𝑗 ... 45

Figure 1.9: (a) 𝐽 path integral with contour (𝛤) looping the crack front, and local co-ordinate system (𝑥𝑖), (b) the virtual crack front extension 𝑞(𝑠), inset shows the

crack extension area Ac, and ∆𝑎, the maximum 𝑞value on ∆𝑠. ... 47 Figure 1.10: Solid shape loaded on boundary 𝑆𝑓 and fixed by displacements on boundary

𝑆𝑢 ... 51

Figure 3.1: The stages of outlier identification: (a) experimental in situ loading with artifact, (b) acquisition of full-field displacements using DIC or DVC and definition of the mask (c) FE discretization showing forces at internal nodes and on the boundary of the domain Ω ... 63 Figure 3.2: Geometry of a human femur generated by (a) geometry-based and (b)

voxel-based meshing strategies. Image from Lengsfeld et al. (1998) ... 63 Figure 3.3: Nodal information in ROI of deformation field ... 65 Figure 3.4: Cantilever beam with artifact locations at α, β (gaussian width σ) and random

noise over the domain Ω ... 69 Figure 3.5: (a) Material distribution with boundary constraints, (b) displacement field

amplitude contour plot showing noise components α and β, and random noise over the entire ROI Ω Locations and dimensions shown in Figure 3.5. ... 69

Figure 3.6: Cross-plot of Equation (3.14), with mean (solid) and 99 % confidence (dashed) ... 69 Figure 3.7: (a) Internal energy during iterations k between (b) the systems transition from

initial to final energy ... 70 Figure 3.8: (a) artifact removal from region of interest of the cantilever showing

magnitudes of force |𝑓| and displacement |𝑢|, threshold at iteration 𝑖= 10 ... 70
Figure 3.9: (a) Arcan fixture and specimen inclined by 30o_{ loaded vertically, (b) }

corresponding region of interest (ROI) showing speckle pattern and unreliable regions (red overlay) ... 71 Figure 3.10: Artifact removal from region of interest of the Arcan specimen (ROI, Figure

3.9) showing magnitudes of force |𝑓| and displacement |𝑢|, predicted to

converge at iteration 10 Note: colour bar axis is rescaled in each iteration. .... 72 Figure 3.11: (a) Incremental quantities from DIC measurements of the ROI of the

inclined crack, (b) Energy increments between initial and final states, ... 73 Figure 3.12: The X-ray facilities with specimen in place and translation stage shown (a),

specimen geometry (b), rendering of the specimen surface using correlation coefficient ... 73 Figure 3.13: (a) Energy increments between initial and final states (top), together with

incremental quantities (bottom) from region of interest of the inclined crack DIC measurements ... 74 Figure 3.14: Artifact removal from region of interest of the Magnesium specimen (ROI,

Figure 3.12b) showing magnitudes of force |𝑓| and displacement |𝑢|, Note: axes are rescaled in each iteration, predicted to converge at iteration 28 ... 74 Figure 4.1: Surfaces (𝑆) defining the surface-volume integral and the volume integral over

crack front segment ∆𝑠. Surfaces with subscripts 0 and 1 define volumes 𝑉0 and 𝑉1 respectively, 𝑆𝑎 and 𝑆𝑏 are the end-caps and 𝑆𝑐 includes the upper and

lower crack faces for 𝑉0 and 𝑉1. ... 79 Figure 4.2: Illustration of the surface-volume integral (Js-vol), the tube-volume integral

(Jhyb), and the classical volume integral (Jvol), with 𝑄 functions and derivatives shown ... 83 Figure 4.3: FEM mesh showing (a) boundary conditions and crack front (0→1), (b) surface

mesh, and (c) banded crack region ... 84 Figure 4.4: (a) 𝐽 results obtained from finite element obtained kinematic fields, (b) showing

only the error from a, (c) 𝐽-values obtained after introducing noise, (d)

showing only the error from c ... 85 Figure 4.5: 𝐽-integral errors due to positional errors ... 86 Figure 4.6: Comparison of 𝐽-integral total errors from displacement noise and positional

errors ... 86 Figure 5.1: 𝐽 line integral, contour path (𝛤), and local (crack tip) co-ordinate system (𝑥𝑖) 92

Figure 5.2: 𝐽 area integral, contour path (𝛤0, 𝛤1, 𝛤+, 𝛤−), crack tip local co-ordinates and 𝑄 function schematic ... 94

Figure 5.3: Schematic of data range and contour selection (𝛤, or A ) for analytical field data, showing: contour position (𝑟𝑐), region of crack influence (𝑟𝑖), and area

integral width (𝐷). ... 96 Figure 5.4: 𝐽-integral results from mixed-mode I-III displacement fields as a function of

contour distance from the crack tip (𝑟𝑐) ... 97

Figure 5.5: KI-III errors due to % displacement noise from line (a) and area (b) integral methods, with SIFs obtained from pure mode I-III fields (i.e. without

decomposition) shown by dashed lines ... 99 Figure 5.6: K estimate % error related to rigid body rotation (a) and off-axis translation in

the 𝑥2 direction (b) ... 100 Figure 5.7: KI-III estimate errors at various contour positions (𝑟𝑐) and a fixed mask width

(𝑟𝑖 = 3 mm) (a), and variable mask width with fixed contour position (b).

Arrows indicate corresponding data points between (a) and (b). Vertical dotted line in (a) indicates the extent of masking (3 mm) ... 100 Figure 5.8: KI-III estimate errors using polynomial interpolation to replace masked data: at

various contour positions (𝑟𝑐) and a fixed mask width (𝑟𝑖 = 3 mm) (a), and

variable mask width with fixed contour position (b) ... 101 Figure 5.9: Arcan specimen geometry (a), schematic of Arcan fixture showing mode I-III

loading directions (b), mounted specimen inclined 30° showing DIC analysed regions (c), and mixed-mode displacement field resulting from DIC analysis (shown on corrected image) (d). ... 103 Figure 5.10: Typical Arcan test setup in 45° mixed-mode loading ... 103 Figure 5.11: KI-III estimates for pure mode I, II and III loading (a-c) Note: mode III loading is applied by 𝑥3 deflection = 3 mm ... 104 Figure 5.12: KI-III estimates normalised to KIc-IIIc, compared to analytical SENT solutions

inclined at 30° (KI-II eq SENT) ... 105 Figure 6.1: Hybrid integral 𝑉 at 𝑠and crack front segment ∆𝑠on the 3D linear crack front

𝑙(𝑠), with inner and outer surfaces (respectively, 𝑆0 and 𝑆1), volumes (𝑉0 and 𝑉1), and virtual crack extension fields (𝑄0 and𝑄1) ... 112 Figure 6.2: (a) Hybrid integral integration volume (𝑉) and (b) cross-section (𝑝-𝑝) showing

contour position 𝑟𝑐 centred between the minimum and maximum contour

positions, 𝑟0_{ and }_{𝑟}1_{, with outer volume width }_{𝐷}_{ ... 113}
Figure 6.3: Hybrid volume integral compared with domain integral and true 𝐽-integral

values ... 114
Figure 6.4: Percentage error in 𝐽 values from random displacement noise ... 114
Figure 6.5: 𝐽 % error due to rotation about axes 𝑥i (𝛾i). ... 116
Figure 6.6: Normalised 𝐽 values determined from mixed mode data (KI = 1 MPa.m1/2_{, }

KII = KII = 0), direction of increasing mask size indicated ... 117
Figure 6.7: Normalised 𝐽 values determined from mixed mode data (KI-III = 1 MPa.m1/2_{), }

Figure 6.8: Comparison of 𝐽 results from the volume, hybrid volume, and equivalent 2D integral at fixed contour position (𝑟𝑐 = 50 %), for increasing mask 𝑟m ... 118

Figure 6.9: Normalised 𝐽 values determined from mixed mode data (KI-III = 1 MPa.m1/2_{), }
replaced by linearly interpolated crack face data, direction of increasing mask
size indicated ... 118
Figure 6.10: Crack front described by discrete points on the crack front sl_{, global crack }

segment co-ordinate system𝑥l_{𝑖}_{, and local co-ordinate system }_{𝑥}l_{ ... 119}
Figure 6.11: (a) Specimen and notch dimensions in global co-ordinate system, (b) X-ray

tomograph of V-notch showing copper particles (light dots) and subset size
(1203_{ voxels), (c) FEM model with crack tip shown expanded. ... 122}
Figure 6.12: Crack front increments showing regions of interest ... 123
Figure 6.13: 𝐽 hybrid volume integral estimates, including the volume integral estimates

(Abaqus) and the SENT analytical estimate in plane strain ... 124 Figure 6.14: Convergence plots for 𝐽-integrals evaluated at positions nearest to (1/2), (2/3) and (4/5) of the crack front. Note: (a), (b), and (c) refer to labels in Figures and 6.16. ... 125 Figure 6.15: (a) Grain boundaries revealing precipitates in WE43 alloy Magnesium using

aqueous saturated picric acid with HCL and a wetting agent, (b) X-CT scan of
sample showing subset size and notch. Note: the notch width apparent in (b) is
50 % greater than the true notch width (0.3 mm) due to the acute angle (30o_{) }
between the notch and cross-section planes. ... 126
Figure 6.16: (a) Inclined notch dimensions, (b) 𝐽-integral evaluations ... 126
Figure 6.17: Normalised 𝐽 hybrid volume integral estimates, including the volume integral

estimates (in-house FEM) and the SENT analytical estimate in plane strain 127 Figure 6.18: 𝐽 values along the crack fronts at position annotated in 7.18-19 ... 128 Figure 7.1: K values estimated from the mid-plane of finite element results, decomposition into mode I, II and III components. ... 135 Figure 7.2: Decomposition into symmetric (mode I) and anti-symmetric (modes II and III)

components ... 136 Figure 7.3: Analytical displacement fields including higher order terms ... 137 Figure 7.4: Decomposition of JAS by obtaining RAS using (a) the stress ratio and (b) the

interaction integral method - mode I results (KI) remaining unchanged. ... 142 Figure 7.5: Contour plots for the interaction integral method (+) and the stress ratio method

(o). ... 142 Figure 8.1: Crack propagation in double-torsion loaded polygranular graphite; (a) loading

rig and sample; (b) extracted image containing ring artifacts; (c) removal of artifact, and non-linearities on the ring and border (NL) ... 147 Figure 8.2: 𝑄 function amplitude on the material surface (left), with possible out of plane

## List of tables

**Page **

Table 1.1: Summary of 𝐽-integral forms and original developers ... 43

Table 1.2: Information assumed to be available in the inverse problem ... 50

Table 3.1: Algorithm for outlier detection and removal ... 68

Table 5.1: Algorithm for field generation ... 98

Table 5.2: Algorithm for error analysis ... 98

Table 5.3: Comparison of fracture toughness values ... 104

## List of abbreviations

2D Two-Dimensional

3D Three-Dimensional

ASTM American Society for Testing and Materials

BEM Boundary Element Method

COD Crack Opening Displacement DIC Digital Image Correlation

DLS Diamond Light Source synchrotron (United Kingdom) DVC Digital Volume Correlation

EPFM Elastic-Plastic Fracture Mechanics EPRI Electric Power Research Institute

ESKOM Electricity Supply Commission (of South Africa)

FE Finite Element

FEM Finite Element Method FFT Fast Fourier Transform

IARE Incremental Artifact Relaxation Energy LEFM Linear Elastic Fracture Mechanics PMMA Polymethyl Methacrylate

ROI Region of Interest

RMSE Root-Mean-Square-Error

SA South Africa

𝑆𝐹 scale factor

SIF Stress Intensity Factor SNR Signal-to-Noise Ratio UCT University of Cape Town

UK United Kingdom

## Nomenclature

a Length of a flaw∆𝑎 Maximum value of the virtual crack extension on the crack front

𝑐𝑛 Co-efficient of strain

𝑓_{𝑀}(𝑛)_{𝑖𝑗} Co-efficient of stress
𝑓_{𝑖} Nodal forces

𝑓̂ Vector of normalized force magnitudes

𝑔𝑖𝑗 Stress function for the virtual fields method

𝑙 Crack front position

𝑛 Order of terms within the Williams series expansion

𝑛_{𝑗} Outward unit normal for the 𝐽-integral

𝑝-𝑝 2D cross-section of 3D volume

𝑞 Virtual crack front extension

𝑟 Radial distance from the crack tip

𝑟_{𝑐} Contour position (rectangular)

𝑟𝑖 Region of crack influence (rectangular)

𝑟𝑘 Radius of 𝐾-dominance

𝑟_{𝑚} Region of mask (rectangular)

𝑠 Crack front position parameter

𝑠𝑙 _{Discrete crack front segment }

∆𝑠 Crack front segment length

𝑢_{𝑎𝑐𝑐} Image correlation displacement accuracy

𝑢_{𝑐𝑟𝑎𝑐𝑘} Crack tip displacements

𝑢𝑒𝑟𝑟 Full-field displacement errors

𝑢𝑖 Displacement field

𝑢_{𝑖,𝑗} Displacement gradients

𝑢_{𝑀} Decompositions for crack tip displacements

𝑢_{𝑝𝑟𝑒𝑐} Experimental precision

𝑢𝐴𝑆 Anti-symmetric component of displacement

𝑣 Poisson's Ratio

𝑥_{𝑗} Local co-ordinate system

𝑥̃_{1}𝑙 _{Global crack segment co-ordinate system }

A Area integral domain

𝐴_{𝑐} Virtual crack extension area

AM Mode (𝑀 = 𝐼, 𝐼𝐼, 𝐼𝐼𝐼) coefficients of the Williams series 𝐶 Correlation coefficient

𝐶𝑁𝐶𝐶 Normalized cross-correlation coefficient

𝐶_{𝑖𝑗}𝑅 Rotation matrix

𝐶_{𝑖}𝑇 _{Rotation vector }

𝐷 Area integral width

𝐸 Young's Modulus

𝐸_{𝑖𝑗} Cauchy stiffness tensor

𝐸∗ _{Nodal Young’s modulu}_{s }

𝐸𝑙 Young’s modulus of a single finite element

𝐸𝑚𝑖𝑛 Young’s modulus of void material

𝐸′ _{Young’s modulus for plane strain or stress}

𝐹 Reference image

𝐹̅ Mean pixel intensity of reference image

𝐹∗ _{Reference image after deformation }

ℱ Fast Fourier Transform (FFT)

ℱ̌ Fast Fourier Transform followed by a complex conjugate operation

ℱ−1 _{Inverse Fast Fourier Transform }

𝐺 Strain energy release rate

𝐽_{𝑎} Area component of the path-area 𝐽-integral

𝐽_{𝑝} Path component of the path-area 𝐽-integral

𝐽_{𝑝𝑎} Path-area integral

𝐽𝑤−𝑝𝑎 Weighted path-area integral

𝐽_{𝑣𝑜𝑙} Volume 𝐽-integral

𝐽(𝑘) 𝐽-integral vector

𝐽_{𝐴𝑆} Antisymmetric component of 𝐽
𝐽𝑆 Symmetric component of 𝐽

𝐽_{𝑆𝐸𝑁𝑇} 𝐽 for the standard Single-Edge-Notch-Test geometry

𝐽_{ℎ𝑦𝑏} Hybrid 𝐽-integral

𝐽𝑀 Modal component of 𝐽 (𝑀 = 𝐼, 𝐼𝐼, 𝐼𝐼𝐼)

𝐽𝑡ℎ Theoretical value for 𝐽 from analytical solution

𝐽 = 𝐽(1) _{𝐽}_{-integral scalar assuming }_{𝑥}_{1}_{ direction crack growth (}_{𝑘 = 1}_{) }

𝐽_{𝐼} Mode I component of 𝐽
𝐽𝐼𝐼 Mode II component of 𝐽

𝐽_{𝐼𝐼𝐼} Mode III component of 𝐽
𝐾_{𝐼} Mode I stress intensity factor

𝐾𝐼𝐼 Mode II stress intensity factor

𝐾𝐼𝐼𝐼 Mode III stress intensity factor

𝐾_{𝐼𝑐} Mode I fracture toughness

𝐾_{𝐼𝐼𝑐} Mode II fracture toughness

𝐾𝐼𝐼𝐼𝑐 Mode III fracture toughness

𝐾_{𝑙}𝑡 _{Template stiffness matrix }

𝐾_{𝐽} Stress intensity factor determined by the 𝐽-integral approach

𝐾_{𝑀} Modal 𝐾 value

𝑀 Mode

𝑁 Total number of nodes of points in DVC or DIC

𝑃′ _{Reflected position of a point }

P∗ _{Displaced position of a point }

𝑄 Virtual crack extension field

𝑄𝐹 Replacement factor for outlier removal

𝑄_{ℎ𝑦𝑏} Hybrid virtual crack extension field

*RAS* Antisymmetric ratio

S Surface

𝑆𝑎, 𝑆𝑏 volume integral end-caps

𝑆𝑐 volume integral crack faces

S_{f} Surface over which a traction is applied

Su Constrained surface

𝑇_{𝑗} Traction on the surface

𝑈 Elastic stored energy

𝑈_{𝑒𝑥𝑡} External energy

𝑈𝑖𝑛𝑡 Internal energy

𝑈_{𝑛} Potential energy due to random errors

𝑈_{𝑜} Portion due to outliers

𝑈̃ Energy residual due to displacement errors

𝛿𝑈̃𝑅𝑀𝑆𝐸 Root-mean-square-error relaxation energy

𝑉 Volume

𝑊 Strain energy density

𝑋𝑖 Global co-ordinate system

𝑌 Crack geometric factor

### Greek symbols

𝛾𝑖 Rotation about the 𝑥i axis [degrees, °]

𝛿_{𝑖𝑗} Kronecker-delta

𝜀_{𝑖𝑗} Strain tensor

𝜀_{𝐴𝑆𝑖𝑗} Anti-symmetric strain components

𝜀_{𝑀𝑖𝑗} Strains for mode 𝑀 = 𝐼, 𝐼𝐼, 𝐼𝐼𝐼
ε_{0} Strain at yield

𝜃 Angle theta [degrees, °]

𝜅 Bulk modulus

𝜌 Density distribution of a material

𝜌_{𝑙} Density of a single finite element

𝜎_{𝑖𝑗} Cauchy stress tensor

𝜎_{𝐴𝑆𝑖𝑗} Anti-symmetric components of the Cauchy stress tensor

𝜎𝑐𝑟𝑎𝑐𝑘 Crack tip stresses

σ_{𝑓𝑓} Stress of the field far from the crack tip region

𝛤 Contour of the line integral

𝛤+_{, }_{𝛤}− _{Contour path coinciding with the upper and lower crack faces }
𝛤0, 𝛤1 Inner and outer boundary contours

∇ First-order gradient of the deformed image Ω Domain of outlier removal

1

## Background reading

Compared to classical solid mechanics, fracture mechanics is still a relatively new field. As
man-made structures have increased in size, it has become increasingly clear that failures
could still not be explained or wholly prevented by solid mechanics principles applied to
constituent parts. Fracture mechanics principles neglect the larger structure, focusing instead
on the notion that failure can be fully characterised by the deformations and loading of the
crack tip, regardless of location. Therefore, the fracture mechanics methodology can be
conveniently applied to laboratory tests, as well as full-scale structures. The proving grounds
for these theories are remembered in the shadow of several catastrophic structural failures in
the 1940s and 1950s that mystified the engineering communities of the decade1_{ (Wells, }
1955).

The modern engineer has a wide array of tools to more fully understand material
performance: numerical methods can simulate the deformation of large structures *in silico*,
and accurate experimental techniques have become available to directly monitor material
deformation across the full-field of the material surface or volume. The latter can be achieved
in an accessible and versatile manner through image correlation.

However, there is a significant gap dividing the numerical modelling and experimental techniques used for the task of fracture characterisation. This thesis aims to bridge this gap, utilising image correlation techniques across the full-field of the surface and volume, and feeding into mathematical derivations of the 𝐽-integral to characterise fracture. The synthesis of these experimental and numerical approaches can then be directed towards gaining a better understanding of fracture in novel materials and structures.

This has applications in two main spheres. Firstly, conventional fracture mechanics allows for the direct assessment of structural integrity through non-destructive estimation of the crack tip parameters (for example, through quantification of crack tip stress fields, or energy release rate approaches such as the 𝐽-integral). Secondly, the techniques are applicable to laboratory tests aiding in the development of new fracture-resistant materials.

Recent trends, described in academic journals such as *Strain*2_{, }* _{Fracture}*3

_{, and }

_{Experimental }*Mechanics*4_{, have been to combine full-field optical measurements with established }
numerical methods to characterise deformations and damage – often referred to as ‘photo
-mechanics’ due to the optical component. Recent developments in this area has been spurred
on by advances in digital image correlation, which provide deformation data from the
full-field of the material with great versatility, as the images can be acquired from transmission

1_{ The two famous examples are the Liberty ships, and the Comet aircraft failures. The Liberty ships, used for }
transport of supplies from the United States to Great Britain during World War II featured an all-welded steel
hull as a replacement to the *de facto* riveted panels. The square corners of the hatch doors acted as stress
concentrations and initiation sites for cracks. Without riveted joints, cracks could propagate unchecked. In 10
cases failure resulted in clean separation of the ships into two-halves, often in calm waters. The Comet jet

aircraft was the world’s first commercial passenger jet, considered state-of-the-art at the time. In 1954 several Comets experienced catastrophic hull loss during routine flight within a three-month period. By replicating flight conditions on the remaining grounded planes, Engineers found that mirco-flaws initiated at pop-rivet sites would propagate due to the regular pressurising and depressurising of the cabin. The final failure initiated near the corners of square cabin windows, which acted as stress concentrators.

2_{ Strain ISSN, online: 1475-1305 }

3_{ Fracture ISSN, print: 0376-9429; online: 1573-2673 }

electron microscopy, neutron diffraction and X-ray computed tomography. This new branch of methods provides the potential to perform online assessment of structures while inspection of the micro-scale and within the volume can lead to a better understanding of the mechanisms that drive them toward fracture.

This doctoral project grew from two earlier projects: the MSc work of the author on
non-destructive testing (Eddy-current detection of fatigue cracks – Molteno, 2012) and the
doctoral work of Becker (2012). The vision was formed that the post-detection monitoring
and analysis of cracks could be achieved by extracting fracture parameters directly from the
fracture site, within a single framework. The approach of Becker *et al.* (2012), achieved this
without prior knowledge of the crack tip position using the 𝐽-integral approach and
two-dimensional (2D) measurements. This provided the impetus to extend the framework to more
general three-dimensional (3D) geometries, and crack orientations.

The following doctoral work commenced in 2013 at Stellenbosch University, with a two year investigation into fracture parameter extraction from regular (white light) images of the surface using image correlation (work summarised in Molteno and Becker, 2015c. The extensions to the volume were developed at Oxford University during 2015 under the auspices of Prof. James Marrow (Department of Materials Science), and using X-ray imaging facilities: MXIF (Manchester University), Diamond Light Source (DLS), to image the volume, including image data-set contributions from Stellenbosch University and Poitiers (France).

The aim of this thesis is therefore to present a framework for the analysis of the 𝐽-integral on the surface, and within the volume using image correlation, but also to enable the extraction of fracture parameters.

1.1

## Project background

Structural survivability is a growing concern in South Africa (SA), brought to light by the
nationwide power shortages and load shedding since 2008 (Bazilian *et al.*, 2012). The
fast-rising demand for electrical energy in SA has forced suppliers to exceed the original
operational lifetimes of over 70 % of coal-fired power plants (Figure 1.1), which still
generate 68 % of the country’s electricity. Eskom, the primary power utility in SA, and
various government agencies have committed to addressing these shortages through various
programmes and incentives. These include large capital investments into coal, gas and
various renewables, aiming to add 12 GW of generating capacity by 2020 (Jestin *et al.*,
2014).

This transition period has placed great importance on the reliability of existing stations as
they see South Africa into a new era of robust electricity supply and economic growth
(Trollip *et al.*, 2014). Therefore, effective structural integrity management has become an
important short and long-term national goal. A significant limitation is that quantitative
damage or fracture estimates are mainly replicated in laboratory controlled tests (Jestin *et *
*al.*, 2014; Scheepers *et al.*, 2010). Such tests seldom reproduce plant conditions (e.g. high
temperatures, cyclic loads, corrosive contact), which are known to aggregate and accelerate
damage (Bezuidenhout, 2010). This results in uncertainty in the extracted parameters,
over-conservatism in component design, ultimately resulting in errors in life estimates on
in-service plant components.

### Figure 1.1: Life expenditures of the current coal-fired Eskom power plants (Molokwane, 2014)

To increase expertise in this area, Eskom launched the Eskom Power Plant Engineering
Institute (EPPEI) programme in 2012 (Jestin *et al.*, 2014), which included a specialisation
in damage characterisation and the prediction of residual component life. Several projects in
damage measurement and monitoring are presently underway as part of a collaboration
between the Material Engineering centres at the University of Cape Town and Stellenbosch
University. Projects at Stellenbosch University have included accelerated creep damage
characterisation (van Rooyen, 2016) and the measurement of fracture parameters from small
sample tests (Huchzermeyer, 2017). Numerous complementary projects have also been
conducted at the University of Cape Town, and can be viewed on the EPPEI Materials
Science and Mechanics Specialisation website5_{. These projects have similar aims: to feed }
into the component service-life management programme currently established at Eskom.
The current Eskom programme seeks to firstly locate damage, and then determine the risk
levels so that high-risk components can be elevated to more in-depth evaluation (e.g. detailed
modelling of bolted joints to determine joint stiffness and contact stresses). The programme
involves non-contact inspection to detect all forms of aberrations (e.g. ultrasonic testing,
eddy current testing), followed by manual dimensioning and monitoring of detected damage
(e.g. by metallographic replication of the surface microstructure), in order to determine the
risk of failure of individual components.

These methods are well established to detect and measure surface and near-surface defects, but are subject to numerous equipment and operator specific limitations when large surface areas must be covered, and objective measurements are required.

1.2

## Full-field measurements with image correlation

Optical full-field measurements in the field of experimental mechanics refers to a collection of techniques, which measure deformation over the full surface or volume of the object from

5_{“}_{Eskom EPPEI}_{”, }_{University of Cape Town, www.mateng.uct.ac.za/mateng/industry/eskom-eppei (accessed }
19 June 2017)

recorded images. Early methods, based on incoherent6_{ light, required separate gratings for }
each deformation state (e.g. moiré (Hareesh and Chiang, 1988)). Various coherent light
based methods have since been developed including holographic interferometry (Kreis,
2005), electronic speckle interferometry (Jacquot Pierre, 2008) and moiré interferometry
(Post, 1991). Although these methods provide high spatial resolution (two orders of
magnitude more independent data-points than DIC), they also require specialised equipment
and complex sample preparations.

As a result, white-light based methods have become increasingly popular for experiments in
which precision can be traded-off for a simpler experimental setup. The two most
well-known white light methods are the grid method, and Digital Image Correlation (DIC)
(Grédiac *et al.*, 2016). The grid method is based on the processing of predetermined patterns,
which are required to be as regular as possible and therefore some sample preparation is
required. Conversely DIC involves the processing of random patterns. Although the pattern
quality has been shown to influence accuracy (Bossuyt, 2013; Schreier *et al.*, 2009), the
method is generally less prescriptive in terms of sample preparation. For instance, random
patterns occur naturally in many materials (e.g. due to grain structure or porosity), and so
the amount of sample preparation is often left to the discretion of the experimentalist.
DIC differs from other optical flow-based methods in that it focuses on the high accuracy
needed in engineering problems to study strains in stiff structures (typically 50-100 µm/m).
This typically leverages assumptions of the materials mechanics, such as continuity and
limited volume change7_{. }

The approach has extensions to multiple cameras, called stereo-DIC; and can be applied
within the volume when volumetric images are available (e.g. via X-ray based imaging),
called Digital Volume Correlation (DVC). These approaches are termed full-field8
techniques because they can obtain deformation data from the entire surface or volume
within the field of view of each image captured. The use of digital images results in a method
that is intuitive (phenomena can often be verified visually by the user) and cost effective
while remaining more accurate and objective than manual measurements. The popularity of
image correlation is apparent from the large body of literature (see for example the review
by Pan *et al.* (2009)) and the growing attention received by these methods in industry (Feng

*et al.*, 2015).

1.3

## The role of fracture mechanics in damage evaluations

Damage quantification is a broad field requiring precise understanding of both the material and environmental parameters of micro and macro length scales. Although damage originates from the microstructure of the material (from physical mechanisms such as creep and fatigue), it is generally first identified as an aggregated effect on the material surface in relatively late stages of damage evolution.

6_{ Coherent light is defined as containing electromagnetic waves, which are in phase with a plane normal to }
the beam direction. Conversely, incoherent light is out-of-phase with the orthogonal plane. Coherent light is
commonly produced for practical purposes by a laser, or when studies in the volume require high-energy rays
a synchrotron is used.

7_{ Contrastingly, another optical technique called Particle Image Velocimetry (PIV) involves loosely }
connected regions to allow for the random rearrangement of particles in fluid flow.

8_{ Also, historically, to discern from point-wise measurements (for example using extensometers and strain }
gauges), upon which there has been great reliance.

Although significant changes in the design properties may occur during the aging of a
material, non-destructive tests tend to be most sensitive to physical defects (e.g. fracture and
void growth). As a result, structural integrity assessment is typically an upstream procedure
starting from the detection of cracking requiring an estimation of short-term risks, towards
an understanding of the underlying damage mechanisms and long-term life predictions.
Short-term risks are often assessed based on Linear Elastic Fracture Mechanics (LEFM)
parameters which describe the fracture toughness of the material. The task of non-destructive
testing and evaluation is then to estimate the subcritical values for such parameters from
components while *in situ*, and compare them to the material limits provided by
manufacturers or *ex situ* tests (e.g. using standards such as ASTM (2015)). This requires a
method to estimate the strain energy release rate (𝐺); the energy released per unit
advancement in crack area.

However, such approaches are typically based on planar deformations and loadings and
standard sample geometries, whereas the geometry of plant components are generally
diverse and three-dimensional. These effects cause complex 3D loading on the crack tip,
which strongly influence crack growth directions (Richard *et al.*, 2005) and the prediction
of ultimate failure (Richard *et al.*, 2014). In LEFM these conditions can be delineated as the
superposition of three distinct modes of fracture (I, II and III, elaborated in section 2.2.1).
Fracture characterisation in the mixed-mode framework requires that 𝐺 is obtained or
separated into its modal components (𝐺𝐼, 𝐺𝐼𝐼, and 𝐺𝐼𝐼𝐼, written 𝐺𝐼−𝐼𝐼𝐼), which can be related

under LEFM assumptions to equivalent stress intensity factors 𝐾_{𝐼−𝐼𝐼𝐼}. The resulting 𝐾_{𝐼−𝐼𝐼𝐼}

factors are the most widely-used fracture parameters in theoretical, numerical and structural integrity analysis (LEFM theory given in section 2.2.3).

The JMAN method by Becker *et al.* (2012) demonstrated that 𝐺 could be estimated directly
from DIC displacement fields using the 𝐽-integral without prior knowledge of the crack tip
position. This characteristic facilitated the study of micro-crack nucleation and the rising
R-curve behaviour in nuclear grade graphite (Becker *et al.*, 2011). JMAN has also been
extended to a resourceful approach in which 𝐺 is computed from neutron diffraction based
strain maps, enabling the direct estimation of 𝐺 without plastic contributions (Barhli *et al.*,
2016). However, the JMAN framework was developed for planar problems, and has
therefore been limited to linear regions in surface experiments (Becker and Tait, 2013),
although the constitutive methods (𝐽-integral, finite elements) are well established in
non-linear materials (Rice and Rosengren, 1968; Kolednik *et al.*, 2014; Yoneyama *et al.*, 2014)
and the volume (Shih *et al.*, 1986).

1.4

## Summary of aims

This project aims to extend the 𝐽-integral framework to 3D, both on the surface and within the volume, that allows for efficient and accurate extraction of mixed-mode fracture parameters (𝐺𝐼−𝐼𝐼𝐼, 𝐾𝐼−𝐼𝐼𝐼) in the volume. The aim is to move away from a finite element

framework, prescribed in the original JMAN approach, to allow for direct application to
stereo-DIC (in- and out-of-plane measurements) and DVC data while remaining versatile
and accessible for future research on mixed-mode behaviour observed in digital images. As
such, the capability to extract mixed-mode stress intensity factors from 𝐺 estimates is seen
as essential: firstly, for providing a quantitative damage assessment tool in the context of
national energy security in light of the forecasted energy requirements (Jestin *et al.*, 2014);
and secondly, to enable mixed-mode analysis in the volume to study damage mechanisms.
These aims are developed further in Chapter 3.

Although it is beyond the scope of this thesis, the hope is that this work will assist in the adoption of full-field measurement techniques as a standard testing practice in structural integrity assessments and lead to better informed maintenance and inspection schedules.

1.5

## Details of thesis layout

The chapters of this thesis concern the various stages of the experimental-numerical methodology to extract 𝐺 and stress intensity factors from stereo-DIC and DVC displacement fields. The intention of this section is to explain the philosophy of the document and to provide suggestions to the reader, who may prefer to read the chapters in a different order.

The results chapters (4-8) have been presented in paper format, as these chapters are either published, in-press or due to be submitted for publication. Therefore, the assistance received from co-authors requires clarification. The convention used in this thesis is to list the contributions in the preamble at the beginning of each chapter. In keeping with this format, each chapter is self-contained. Therefore, this thesis does not contain a single comprehensive literature review, but rather a background reading chapter (Chapter 2) containing broad contextual information on the methods used. The detailed literature concerning each technique can be found in the introduction of each results chapter (4-8).

The techniques introduced in Chapter 2 include: the principles of image correlation and the limitations in terms of spatial resolution close to fracture surfaces, elements of full-field fracture mechanics, the methods to acquire mixed-mode parameters, and some methods to acquire the constitutive properties of materials are presented in brief. This final topic concerns a broad field of inverse problems in experimental mechanics that is not developed elsewhere in this thesis.

Chapter 3 develops the hypothesis of the thesis. Initially the methodology is formulated in terms of the advantages that certain highlighted techniques can achieve with DIC and DVC data (summarised in section 2.4). These are presented in a series of methodology statements. The aim is to focus this thesis on a small number of techniques that can form a complete methodology for practical applications (e.g. with Eskom) at an early stage. The objectives for the development and verification of this methodology are then defined, giving rise to the central hypothesis of the thesis in section 3.3. All following chapters, excluding the final discussion and conclusions (chapters 9 and 10), present the developments of the methodology following the order of the objectives listed in section 3.2.

Chapter 4 introduces a technique for pre-processing displacement fields to locate and remove errors. The techniques in this thesis rely on the capabilities of DIC and DVC in the presence of fracture surfaces, which results in well-known error localisations (discussed in section 2.1) and which are challenging to separate from inherent random errors. This section proposes a framework that minimises such errors in both surface and volume datasets. This chapter is the first results chapter and sets the scene in terms of the limitations of DIC and DVC in fracture problems.

Chapter 5 develops a framework to establish the noise susceptibility of the 𝐽-integral. The framework has a theoretical basis that builds on the generic derivation of the 𝐽-integral provided in the background reading (section 2.2.5). The following chapters (0, 7 and 8) draw on this framework to determine 𝐽 from DIC and DVC displacement data and separate 𝐽

values into separate opening, shearing and tearing (I, II and III) modes to determine stress intensity factors. The procedure in each case (on the surface, within the volume, and in

various discussion sections) always covers the 𝐽-integral method first, and then the decomposition method.

Chapters 0, 7, and 8 introduce the 𝐽-integral based decomposition method starting with displacements on the surface and then in the volume. Chapter 0 introduces and verifies the

𝐽-integral and decomposition method on the surface using DIC data. However, the same
brevity could not be achieved in the volume. Instead, the 3D 𝐽-integral implementation and
testing (Chapter 7) is separate to the decomposition method in the volume (Chapter 8).
To assess the combined methodology developed throughout the thesis, a comprehensive
discussion is included. The objective is to assess the suitability of the proposed techniques
to perform *in situ* measurements from standard DIC and DVC experiments. This section also
contains recommendations for future work and highlights complementary aspects of this
work to the existing approaches used by Eskom. Chapter 10 contains the thesis conclusions,
which highlight the main achievements and novel contributions to the underlying methods
used to achieve the objectives (in section 3.2) of this thesis.

2

## Background reading

The following sections introduce deformation measurement using digital images, the extraction of fracture parameters, and mechanical properties. The methods proposed in this thesis do not acquire all the properties necessary to achieve fracture parameter estimation, as discussed in the scope section (section 3.4). Therefore, certain topics – too relevant to omit (e.g. 2.2.4, 2.3) – have been included for a more complete picture.

2.1

Image correlation

Digital Image Correlation (DIC) as referred to in the thesis title, typically refers to 2D images. However, the same principles have been established in 3D both on the surface using multi-camera setups (called stereo-DIC), and in the volume using Digital Volume Correlation (DVC). Note that appart from the dimensional extension, the principles of both DIC and DVC are identicle. Therefore, for simplicity of presentation, the following sections assume 2D deformations (i.e. DIC analysis) as a starting point.

### 2.1.1 Overview of principles

DIC was first established in the early 1980s as a versatile alternative to traditional
extensometry (Peters and Ranson, 1982; Sutton *et al.*, 1983; Chu *et al.*, 1985; Sutton *et al.*,
1986). The method enables the processing of digital images captured both before and after
material loading in order to obtain the samples’ deformations (Figure 2.1a). Within areas of
uniform isotropy, displacements can be obtained from arbitrary selections of pixels, or
‘subsets’, over the field of view of the sample. The resulting displacement vectors are thus
able to occupy the ‘full-field’9_{. In practice, users may select parameters (e.g. subset size and }

9_{ The density of displacements is also limited by the principles found in sampling theory such as the }
Nyquist-Shannon rate and the photo-detector grid spacing.

spacing) that are optimal for a particular experimental setup, which may be limited in terms of image quality, or computational resources.

The image correlation procedure may be further explained with the example of a pre-cracked
compact tension specimen, shown in Figure 2.1a. If the specimen surface is parallel to the
camera lens, and if imaging non-linearities can be disregarded (e.g. perspective, lens
distortion), calibration of 2D images involves only the scaling of pixels using a direct
length-to-pixel ratio. This approach is frequently applied at smaller length scales, such as SEM
images (Sutton *et al.*, 2007) or in volumetric imaging (Maire and Withers, 2014). However,
it is often the case that imaging non-linearities cause spurious displacements that require
removal to improve the accuracy of the displacement fields. To achieve this, an object with
a precisely known geometry and high contrast features can be used for calibration. In this
thesis, this approach is needed to account for perspective effects in multi-camera (stereo)
DIC systems, which typically use a stepped calibration plate marked with a dotted or
checkerboard pattern (Schreier *et al.*, 2009). Note that with most calibration strategies, the
displacement data is mapped to the co-ordinate system of the calibration plate. In fracture
mechanics analysis the convention is to align the co-ordinate axes with the 𝑥_{1} axis ahead of
the crack, the 𝑥_{2} axis perpendicular to the crack plane and (in 3D problems), the 𝑥_{3} axis
perpendicular to the surface, or tangential to the crack front in the volume10_{ (Figure 2.1b - }
top image).

To illustrate the problem of image motion, consider the function 𝐹(𝑥𝑖), a grey-level image

with pixel intensity values at positions 𝑥_{𝑖}. Note that the although images only contain
information at the pixel positions, it is assumed that inter-pixel positions can be obtained via
interpolation. Therefore, 𝐹(𝑥_{𝑖}) is a continuous scalar function that can be mapped using a
displacement field 𝑢_{𝑖}, written as 𝐹(𝑥_{𝑖} + 𝑢_{𝑖}). The subscript 𝑖 is 𝑖 = 1,2 for 2D images (DIC)
but extends to 𝑖 = 1,2,3 for 3D (stereo-DIC or DVC). The task of obtaining the deformation
field from a subsequent image 𝐹∗_{ of the deformed object can then be derived from the optical }

flow equation,

assuming ideal mapping conditions (constancy of brightness, exact interpolation, etc.). One
approach is to select a subset of pixels {𝑥_{𝑖}} with local deformation field {𝑢_{𝑖}}. Each subset is
referenced to its centre at location 𝑃 in the reference image (Figure 2.1c). The task is then to
determine the local displacement, rotation, and deformation parameters to optimally match
each subset from 𝑃 to their corresponding positions in the deformed image 𝐹∗_{ at }_{𝑃}∗_{. This is }

achieved when the optical flow is satisfied locally within each subset 𝐹({𝑥_{𝑖}} + {𝑢𝑖}) =

𝐹∗_{({𝑥}

𝑖}) (e.g. between 𝐹 and 𝐹∗ in Figure 2.1b). Numerous approaches to solve Equation

(2.1) have been proposed, including global methods (see section 2.1.3). An efficient and
widely used method to achieve the best match is by linearization of (2.1) and iterative
updating of the displacement field {𝑢_{𝑖}} via Newton’s method (Yates *et al.*, 2010),

10_{ In geometries with curved crack fronts, the axis alignment and mapping of kinematics is often specified }
within the subsequent fracture mechanics technique. Such a strategy is introduced in Chapter 7 to align with
an inclined crack.

𝐹(𝑥_{𝑖}) = 𝐹∗_{(𝑥}

### Figure 2.1: (a) Crack sample (CT specimen) loaded in tension, (b) images from before (top) and after (bottom) loading in the crack tip co-ordinate system, used as the reference and deformed configurations respectively on the surface (c) – schematic (d) shows typical subset

where 𝑛 is the iteration number, ∇ is the first-order gradient of the deformed image, and 𝐹

is the reference image after the 𝑛th_{ deformation }_{𝐹}(𝑛)_{({𝑥}

𝑖}) = 𝐹({𝑥𝑖} + {𝑢𝑖}(𝑛)). The quality

of the match can also be determined directly by formulating a correlation criterion, with
examples including the sum of square differences, Fourier transform based criteria, and
point-wise methods (Jin and Bruck, 2005). A commonly used criterion is the normalized
cross-correlation coefficient (𝐶_{𝑁𝐶𝐶}), expressed as,

in which, 𝐹∗_{ and }_{𝐹}(𝑛)_{ may be optimised globally or over subsets }_{{𝑥}

𝑖}, overbar (𝐹̅) indicates

a mean pixel intensity, and 𝑠𝑠 is the domain of the selected subset. When the correlation
criterion is defined explicitly (e.g. Equation (2.1)), the DIC method relies on a robust and
efficient optimisation algorithm to determine {𝑢_{𝑖}}. In the subset based procedure, image
matching is repeated on a regular grid resulting in a deformation map of the surface (DIC)
or the volume (DVC). In the subset based approach, the user typically optimises the accuracy
by adjusting the subset parameters (e.g. the subset size, spacing or overlap shown in Figure
2.1d), to maximise spatial resolution and accuracy, as discussed further in section 2.1.3. A
study on stress corrosion cracking mechanisms (loading of a submerged fatigue crack in
3.5 % sodium chloride at 90 °C (Becker *et al.*, 2016)) is shown in Figure 2.2a, to illustrate
two limitations of image correlation:

(1) The tracking of features relies on the fidelity and uniqueness of the features across all images captured before and during deformation. Feature fidelity is only considered to be maintained if the contrast patterns of any image can be mapped to match the same feature in all other images of the deformed sample. Such effects are numerous, but are commonly due to damage (e.g. fracture, scratched surface during testing, as shown in Figure 2.2a), foreign particles on the sample or sensor grid, or movement of the sample during image capture.

(2) There is a further requirement for uniqueness of the pattern, often referred to as the
correspondence problem. This effect results from repetitive patterns (see Figure 2.2b),
such as regular grids of dots, or parallel lines. This results in multiple possible solutions
to the pattern matching approach between a reference pattern at position indicated by
position 𝑃, and a pattern translated and deformed to a new position 𝑃∗_{. This problem }

can also be linked to low image gradients, as shown in Figure 2.2c.

{𝑢𝑖}(𝑛+1)= {𝑢𝑖}(𝑛)− (
𝐹∗_{({𝑥}
𝑖}) − 𝐹(𝑛)({𝑥𝑖})
∇𝐹∗_{({𝑥}
𝑖}) )
(2.2)
𝐶𝑁𝐶𝐶 =
∑ [(𝐹∗_{− 𝐹̅}∗)_{) (𝐹}(𝑛)_{− 𝐹̅}(𝑛)_{)]}
𝑠𝑠
∑ {[𝐹∗_{− 𝐹̅}∗_{]}2_{∑ [𝐹}(𝑛)_{− 𝐹̅}(𝑛)_{]}2
𝑆 }
1
2
𝑠𝑠
, 𝐶𝑁𝐶𝐶 ∈ [0,1] (2.3)

### Figure 2.2: Examples of fundamental problems in image matching: (a) loss of pattern fidelity and (b, c) the correspondence problem.

**(a) shows an example of stress corrosion cracking in a laser etched sample from (Becker ****et al.****, **
**2016), (b) is a repeating structure and (c) is a textureless deforming structure. **

Correspondence errors can be reduced by global optimisers (e.g. genetic algorithms (Jin and
Bruck, 2005; Bing and Xie, 2007; Zhao *et al.*, 2012)). However, these approaches are
computationally expensive (Pan *et al.*, 2009).

Another approach which achieves greater efficiency and a wider search range is the
phase-correlation based approach developed by Chen *et al.* (1993). This performs image matching
in the frequency domain, usually calculated by fast Fourier transforms. Due to translation
invariance, 𝐶𝑁𝐶𝐶 correlation values can be determined at each point in {𝑥𝑖} from a single

calculation,

in which ∘ is the entry-wise product11_{, }_{ℱ}_{ and }_{ℱ}−1_{ are the forward and inverse discrete }

Fourier transforms, and ℱ̌ is the forward Fourier transform followed by a complex conjugate operation (change of sign of the imaginary part). The division by the complex modulus |∙|

normalizes the entries in the numerator so that 𝐶𝑁𝐶𝐶 ranges between [0,1] (zero is no

correlation). The displacement is then determined by the location of the peak in 𝐶_{𝑁𝐶𝐶}({𝑥_{𝑖}}).
With this method, correlation values are only available at pixel locations, and so subpixel
accuracy requires interpolation using the neighbourhood of 𝐶𝑁𝐶𝐶 values, for example the

efficient 2×2 method by Foroosh *et al.* (2002). This approach is sensitive to rotation and
scaling. However, such parameters can also be determined in a translation invariant manner
by first converting the reference and deformed images to log-polar co-ordinates (De Castro
and Morandi, 1987; Srinivasa Reddy and Chatterji, 1996). As neither approach solves the
entire set of deformation parameters, iterative updating (e.g. switching between log-polar
and cartesian) is often used to so that the images may be better aligned by interpolation (as
shown by {𝑢𝑖} in Equation (2.4)).

Note that the Fourier transform is also sensitive to non-uniqueness of patterns, particularly
if the pattern is periodic (Schreier *et al.*, 2009). These requirements have led to the
widespread use of random speckle patterns (e.g. spray paint, or air-brush), when the natural
features of the material do not suffice (see example speckle patterns in Figure 2.1 (a) and

11_{ Known more formally as the Hadamard product. }

𝐶_{𝑁𝐶𝐶}({𝑥_{𝑖}}) = ℱ−1 ℱ(𝐹∗({𝑥𝑖}))∘ℱ̌(𝐹({𝑥𝑖} + {𝑢𝑖}))

|ℱ(𝐹∗_{({𝑥}

𝑖}))∘ℱ̌(𝐹({𝑥𝑖} + {𝑢𝑖})|

(b)), or need to be optimised to improve the accuracy of calculated strains (Bossuyt, 2013). Other aspects of accuracy are related to the image correlation parameters, as discussed in the next section.

### 2.1.2 Displacement accuracy and spatial resolution

The accuracy and computational efficiency of image correlation is particularly high if image
regions exhibit low deformation gradients. This allows the selection of large subsets while
maintaining the low order of deformation complexity12_{ (usually linear or cubic basis }
functions are preferred for efficiency). However, a limit is reached when further increases in
subset size yield no improvement, or a reduction in accuracy. This occurs when the subset
contains deformations that do not belong to the space of shape functions of the subset.
Complex deformations are mainly the result of geometric boundaries, damage, complex
loading, and various unwanted artifacts (such as the previously discussed pattern errors in
Figure 2.2). More formally, the spatial resolution, defined as *the shortest distance between *
*two spatially independent measurements* in (Grédiac and Sur, 2014). Therefore, the spatial
resolution is not improved by use of subsets with significant overlaps, but requires a
reduction in subset size.

Due to the complexity of deformation, it is challenging to ascertain the true displacement
errors from deformation experiments. An effective test for DIC or DVC errors is therefore
to rigidly translate the sample (without rotation). It has also been shown that the relationship
between subset size (𝑙) and displacement errors is proportional to 𝑙−1_{ and }_{𝑙}−3/2_{ for DIC }

(Besnard *et al.*, 2006) and DVC (Leclerc *et al.*, 2011) respectively. However, such relations
are difficult to separate from the other parameters linked to the image correlation method
(such as interpolation function and length scale). This has been studied by Yaofeng and Pang
(2007), and optimised by Li *et al.* (2017).

This dilemma is a pertinent issue in fracture measurements, in which a high accuracy is
needed for various approaches to extract fracture parameters (e.g. direct measurements of
crack opening displacement, or displacement extrapolation approaches (Lim *et al.*, 1992)).
The crack tip fields are discontinuous along the crack faces and asymptotic in gradient as
they approach the crack tip, leading to large inaccuracies and failed correlations over the
crack region (as shown previously in Figure 2.1d). Reducing the subset size leads to a
reduction in accuracy in this region, which is worsened if the nonlinear effects of damage
have spread ahead of the crac